Application: All-Terrain Vehicles Brake System Functional Requirements: Structurally intact; Withstand 13.8 Mpa (2,000 PSI) Pressure (proof test) Competing Technology: Machining Overall Size: Overall length 40 mm, bolt retain section 13.5 mm I.D. 2.0 mm, wall thickness as thin as 0.7 mm Part Weight: 11.6 grams (barbed), 15.0 grams (straight) Material: MIM-17-4 PH, H-1100 Heat Treat
Key Requirements: 1. Hermetic at 2,000 psi 2. Free fluid passage in the 2 mm ID 3. Bolt sealing surfaces free of flash and parting line 4. Make both part types in same mold base 5. Reasonable corrosion resistance
2 mm ID for hydraulic fluid passage Contoured, flash & parting-line free sealing surfaces on both sides of 6 mm bolt hole Gate
O.D - 3.4 mm I.D. - 2.0 mm Thin wall on barbed component needed to withstand 2,000 psi & maintain hermeticity.
Interchangeable tooling insert that allows both barbed & straight features to be molded Notch in 6 mm Bolt ID pins (both sides of tool) captures 2 mm ID pin Parting line in center of 6mm bolt hole creates smooth surfaces for crush washers
Why MIM? – 17-4 Material more than adequate for strength & corrosion requirements – 2 mm ID, difficult to machine, is straightforward for MIM (straightness not an issue) – Molded bolt hole surfaces create smooth mating surfaces for crush washers – Both part types easily made in the same tooling – MIM consistency created few problems in production
Conclusion – Application worked well for MIM. – An example of how some of the “easy” attributes of MIM can be very useful to end users